An organic-inorganic hybrid co-crystal complex as a high-performance solid-state nonlinear optical switch
Tianliang Chen; Zhihua Sun; Sangen Zhao; Chengmin Ji; Junhua Luo; Journal of Materials Chemistry C 4 (2016) 266–271; doi:10.1039/C5TC03278D

data_7234525
_publ_section_title
;
 An organic-inorganic hybrid co-crystal complex as a high-performance
 solid-state nonlinear optical switch
;
_journal_name_full               'Journal of Materials Chemistry C'
_journal_page_first              266
_journal_page_last               271
_journal_paper_doi               10.1039/C5TC03278D
_journal_volume                  4
_journal_year                    2016
_chemical_formula_moiety         ' C6 H2 N2, Cl3 Fe H6 O3, 2(Cl)'
_chemical_formula_sum            'C6 H8 Cl5 Fe N2 O3'
_chemical_formula_weight         389.24
_space_group_IT_number           62
_space_group_name_Hall           '-P 2ac 2n'
_space_group_name_H-M_alt        'P n m a'
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_H-M   'P n m a'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   12.7268(6)
_cell_length_b                   17.1535(7)
_cell_length_c                   7.0352(3)
_cell_measurement_temperature    293(2)
_cell_volume                     1535.85(12)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0295
_diffrn_reflns_av_sigmaI/netI    0.0302
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_k_max       21
_diffrn_reflns_limit_k_min       -21
_diffrn_reflns_limit_l_max       8
_diffrn_reflns_limit_l_min       -8
_diffrn_reflns_number            5151
_diffrn_reflns_theta_full        26.37
_diffrn_reflns_theta_max         26.37
_diffrn_reflns_theta_min         3.13
_exptl_absorpt_coefficient_mu    1.847
_exptl_crystal_colour            orange-yellow
_exptl_crystal_density_diffrn    1.683
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       cuboid
_exptl_crystal_F_000             772
_exptl_crystal_preparation       'phase transition'
_exptl_crystal_recrystallization_method
'Re-crystallisation from solvent: water'
_exptl_crystal_size_max          0.20
_exptl_crystal_size_mid          0.20
_exptl_crystal_size_min          0.10
_refine_diff_density_max         0.512
_refine_diff_density_min         -0.766
_refine_diff_density_rms         0.189
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.045
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     115
_refine_ls_number_reflns         1618
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.045
_refine_ls_R_factor_all          0.0497
_refine_ls_R_factor_gt           0.0421
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0798P)^2^+0.9401P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1188
_refine_ls_wR_factor_ref         0.1272
_reflns_number_gt                1390
_reflns_number_total             1618
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            J-Mater-Chem-C-2016-4-266.cif
_cod_data_source_block           1
_cod_original_sg_symbol_H-M      Pnma
_cod_original_formula_sum        ' C6 H8 Cl5 Fe N2 O3'
_cod_database_code               7234525